LMucko/crystallography-open-database huggingface dataset:
Quelques Fluorures Mixtes Terre Rare - Metal Alcalin de Structures derivees de celle de la Fluorine
Aleonard, S; le Fur, Y; Pontonnier, L; Gorius, M F; Roux, M T; Annales de Chimie (Paris) (Vol=Year) 1978 (1978) 417–427; doi:

data_1008041
_publ_section_title
;
Quelques Fluorures Mixtes Terre Rare - Metal Alcalin de Structures
derivees de celle de la Fluorine
;
_journal_coden_ASTM              ANCPAC
_journal_name_full               'Annales de Chimie (Paris) (Vol=Year)'
_journal_page_first              417
_journal_page_last               427
_journal_volume                  1978
_journal_year                    1978
_chemical_formula_structural     'K Er F4'
_chemical_formula_sum            'Er F4 K'
_chemical_name_systematic        'Potassium erbium fluoride'
_space_group_IT_number           151
_symmetry_cell_setting           trigonal
_symmetry_Int_Tables_number      151
_symmetry_space_group_name_Hall  'P 31 2 (0 0 4)'
_symmetry_space_group_name_H-M   'P 31 1 2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            18
_cell_length_a                   14.08
_cell_length_b                   14.08
_cell_length_c                   10.12
_cell_volume                     1737.5
_cod_database_code               1008041
Quelques Fluorures Mixtes Terre Rare - Metal Alcalin de Structures derivees de celle de la Fluorine
Aleonard, S; le Fur, Y; Pontonnier, L; Gorius, M F; Roux, M T; Annales de Chimie (Paris) (Vol=Year) 1978 (1978) 417–427; doi:

data_1008042
_publ_section_title
;
Quelques Fluorures Mixtes Terre Rare - Metal Alcalin de Structures
derivees de celle de la Fluorine
;
_journal_coden_ASTM              ANCPAC
_journal_name_full               'Annales de Chimie (Paris) (Vol=Year)'
_journal_page_first              417
_journal_page_last               427
_journal_volume                  1978
_journal_year                    1978
_chemical_formula_structural     'K Y3 F10'
_chemical_formula_sum            'F10 K Y3'
_chemical_name_systematic        'Potassium triyttrium fluoride'
_space_group_IT_number           225
_symmetry_cell_setting           cubic
_symmetry_Int_Tables_number      225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   11.51
_cell_length_b                   11.51
_cell_length_c                   11.51
_cell_volume                     1524.8
_cod_database_code               1008042
Quelques Fluorures Mixtes Terre Rare - Metal Alcalin de Structures derivees de celle de la Fluorine
Aleonard, S; le Fur, Y; Pontonnier, L; Gorius, M F; Roux, M T; Annales de Chimie (Paris) (Vol=Year) 1978 (1978) 417–427; doi:

data_1008043
_publ_section_title
;
Quelques Fluorures Mixtes Terre Rare - Metal Alcalin de Structures
derivees de celle de la Fluorine
;
_journal_coden_ASTM              ANCPAC
_journal_name_full               'Annales de Chimie (Paris) (Vol=Year)'
_journal_page_first              417
_journal_page_last               427
_journal_volume                  1978
_journal_year                    1978
_chemical_formula_structural     'K Yb3 F10'
_chemical_formula_sum            'F10 K Yb3'
_chemical_name_systematic        'Potassium triytterbium fluoride - $-beta'
_space_group_IT_number           186
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      186
_symmetry_space_group_name_Hall  'P 6c -2c'
_symmetry_space_group_name_H-M   'P 63 m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            4
_cell_length_a                   8.07
_cell_length_b                   8.07
_cell_length_c                   13.2
_cell_volume                     744.5
_cod_database_code               1008043
Quelques Fluorures Mixtes Terre Rare - Metal Alcalin de Structures derivees de celle de la Fluorine
Aleonard, S; le Fur, Y; Pontonnier, L; Gorius, M F; Roux, M T; Annales de Chimie (Paris) (Vol=Year) 1978 (1978) 417–427; doi:

data_1008044
_publ_section_title
;
Quelques Fluorures Mixtes Terre Rare - Metal Alcalin de Structures
derivees de celle de la Fluorine
;
_journal_coden_ASTM              ANCPAC
_journal_name_full               'Annales de Chimie (Paris) (Vol=Year)'
_journal_page_first              417
_journal_page_last               427
_journal_volume                  1978
_journal_year                    1978
_chemical_formula_structural     'K Er3 F10'
_chemical_formula_sum            'Er3 F10 K'
_chemical_name_systematic        'Potassium trierbium fluoride - $-beta'
_space_group_IT_number           8
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      8
_symmetry_space_group_name_Hall  'C -2y'
_symmetry_space_group_name_H-M   'C 1 m 1'
_cell_angle_alpha                90
_cell_angle_beta                 109.45
_cell_angle_gamma                90
_cell_formula_units_Z            16
_cell_length_a                   14.08
_cell_length_b                   8.137
_cell_length_c                   28.28
_cell_volume                     3055.1
_cod_database_code               1008044
Quelques Fluorures Mixtes Terre Rare - Metal Alcalin de Structures derivees de celle de la Fluorine
Aleonard, S; le Fur, Y; Pontonnier, L; Gorius, M F; Roux, M T; Annales de Chimie (Paris) (Vol=Year) 1978 (1978) 417–427; doi:

data_1008045
_chemical_name_systematic          'Potassium trithulium fluoride - $-beta'
_chemical_formula_structural       'K Tm3 F10'
_chemical_formula_sum              'F10 K Tm3'
_publ_section_title
;
Quelques Fluorures Mixtes Terre Rare - Metal Alcalin de Structures
derivees de celle de la Fluorine
;
_journal_name_full                 'Annales de Chimie (Paris) (Vol=Year)'
_journal_coden_ASTM                ANCPAC
_journal_volume                    1978
_journal_year                      1978
_journal_page_first                417
_journal_page_last                 427
_cell_length_a                     20.9
_cell_length_b                     8.2
_cell_length_c                     20.9
_cell_angle_alpha                  90
_cell_angle_beta                   109.5
_cell_angle_gamma                  90
_cell_volume                       3376.4
_cell_formula_units_Z              18
_cod_database_code 1008045
Vacancies ordering in new metastable orthophosphates (Co~3~ ) P~2~ O~8~ and (Mg~3~ ) P~2~ O~8~ with olivin-related structure
Berthet, G; Joubert, J C; Bertaut, E F; Zeitschrift fuer Kristallographie, Kristallgeometrie, Kristallphysik, Kristallchemie (-144,1977) 136 (1972) 98–105; doi:

data_1008046
_publ_section_title
;
Vacancies ordering in new metastable orthophosphates (Co~3~ ) P~2~ O~8~
and (Mg~3~ ) P~2~ O~8~ with olivin-related structure
;
_journal_coden_ASTM              ZEKGAX
_journal_name_full
;
Zeitschrift fuer Kristallographie, Kristallgeometrie, Kristallphysik,
Kristallchemie (-144,1977)
;
_journal_page_first              98
_journal_page_last               105
_journal_volume                  136
_journal_year                    1972
_chemical_formula_structural     'Co3 (P O4)2'
_chemical_formula_sum            'Co3 O8 P2'
_chemical_name_systematic        'Cobalt phosphate'
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2bc'
_symmetry_space_group_name_H-M   'P 1 1 21/b'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                91.07
_cell_formula_units_Z            2
_cell_length_a                   5.92(2)
_cell_length_b                   10.334(30)
_cell_length_c                   4.75(2)
_cell_volume                     290.5
_refine_ls_R_factor_all          0.1
_cod_database_code               1008046
Synthese et structure cristalline d'un nouvel oxyde mixte Fe V~2~ O~6~ H~0.5~. Relation avec la structure type Diaspore
Muller, J; Joubert, J C; Marezio, M; Journal of Solid State Chemistry 27 (1979) 367–382; doi:10.1016/0022-4596(79)90179-8

data_1008047
_publ_section_title
;
Synthese et structure cristalline d'un nouvel oxyde mixte Fe V~2~ O~6~
H~0.5~. Relation avec la structure type Diaspore
;
_journal_coden_ASTM              JSSCBI
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              367
_journal_page_last               382
_journal_paper_doi               10.1016/0022-4596(79)90179-8
_journal_volume                  27
_journal_year                    1979
_chemical_formula_structural     'Fe V2 O6 H0.5'
_chemical_formula_sum            'Fe H0.5 O6 V2'
_chemical_name_systematic        'Iron vanadium oxide hydroxide *'
_space_group_IT_number           19
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      19
_symmetry_space_group_name_Hall  'P 2ac 2ab'
_symmetry_space_group_name_H-M   'P 21 21 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   4.891(1)
_cell_length_b                   9.553(2)
_cell_length_c                   8.786(2)
_cell_volume                     410.5
_refine_ls_R_factor_all          0.024
_cod_original_formula_sum        'H.5 Fe O6 V2'
_cod_database_code               1008047
Structural aspects of the metal-insulator transition in (Ti~0.9975~ V~0.0025~)~4~ O~7~
Hodeau, J L; Marezio, M; Journal of Solid State Chemistry 29 (1979) 47–62; doi:10.1016/0022-4596(79)90208-1

data_1008048
_publ_section_title
;
Structural aspects of the metal-insulator transition in (Ti~0.9975~
V~0.0025~)~4~ O~7~
;
_journal_coden_ASTM              JSSCBI
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              47
_journal_page_last               62
_journal_paper_doi               10.1016/0022-4596(79)90208-1
_journal_volume                  29
_journal_year                    1979
_chemical_formula_analytical     '(Ti0.9975 V0.0025)4 O7'
_chemical_formula_structural     'Ti4 O7'
_chemical_formula_sum            'O7 Ti4'
_chemical_name_systematic        Heptaoxotetratitanate
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1 (-x,-1/2*y+1/2*z,1/2*y+1/2*z)'
_symmetry_space_group_name_H-M   'A -1'
_cell_angle_alpha                95.05(1)
_cell_angle_beta                 95.19(1)
_cell_angle_gamma                108.76(1)
_cell_formula_units_Z            4
_cell_length_a                   5.5942(6)
_cell_length_b                   7.1216(8)
_cell_length_c                   12.460(1)
_cell_volume                     464.5
_refine_ls_R_factor_all          0.025
_cod_database_code               1008048
Structural aspects of the metal-insulator transition in (Ti~0.9975~ V~0.0025~)~4~ O~7~
Hodeau, J L; Marezio, M; Journal of Solid State Chemistry 29 (1979) 47–62; doi:10.1016/0022-4596(79)90208-1

data_1008049
_publ_section_title
;
Structural aspects of the metal-insulator transition in (Ti~0.9975~
V~0.0025~)~4~ O~7~
;
_journal_coden_ASTM              JSSCBI
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              47
_journal_page_last               62
_journal_paper_doi               10.1016/0022-4596(79)90208-1
_journal_volume                  29
_journal_year                    1979
_chemical_formula_analytical     '(Ti0.9975 V0.0025)4 O7'
_chemical_formula_structural     'Ti4 O7'
_chemical_formula_sum            'O7 Ti4'
_chemical_name_systematic        Heptaoxotetratitanate
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1 (-x,-1/2*y+1/2*z,1/2*y+1/2*z)'
_symmetry_space_group_name_H-M   'A -1'
_cell_angle_alpha                95.00(1)
_cell_angle_beta                 95.426(9)
_cell_angle_gamma                109.023(9)
_cell_formula_units_Z            4
_cell_length_a                   5.5943(5)
_cell_length_b                   7.1297(7)
_cell_length_c                   12.484(1)
_cell_volume                     464.9
_refine_ls_R_factor_all          0.031
_cod_database_code               1008049
Structural aspects of the metal-insulator transition in (Ti~0.9975~ V~0.0025~)~4~ O~7~
Hodeau, J L; Marezio, M; Journal of Solid State Chemistry 29 (1979) 47–62; doi:10.1016/0022-4596(79)90208-1

data_1008050
_publ_section_title
;
Structural aspects of the metal-insulator transition in (Ti~0.9975~
V~0.0025~)~4~ O~7~
;
_journal_coden_ASTM              JSSCBI
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              47
_journal_page_last               62
_journal_paper_doi               10.1016/0022-4596(79)90208-1
_journal_volume                  29
_journal_year                    1979
_chemical_formula_analytical     '(Ti0.9975 V0.0025)4 O7'
_chemical_formula_structural     'Ti4 O7'
_chemical_formula_sum            'O7 Ti4'
_chemical_name_systematic        Heptaoxotetratitanate
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_Int_Tables_number      2
_symmetry_space_group_name_Hall  '-P 1 (-x,-1/2*y+1/2*z,1/2*y+1/2*z)'
_symmetry_space_group_name_H-M   'A -1'
_cell_angle_alpha                95.056(2)
_cell_angle_beta                 95.550(5)
_cell_angle_gamma                109.676(5)
_cell_formula_units_Z            4
_cell_length_a                   5.6235(3)
_cell_length_b                   7.1984(4)
_cell_length_c                   12.4018(5)
_cell_volume                     466.6
_refine_ls_R_factor_all          0.022
_cod_database_code               1008050
A new cubic K Sb O~3~ derivative structure with interpenetrating networks. Crystal structure of Bi~3~ Ga Sb~2~ O~11~
Sleight, A W; Bouchard, R J; Inorganic Chemistry 12 (1973) 2314–2316; doi:10.1021/ic50128a019

data_1008051
_publ_section_title
;
A new cubic K Sb O~3~ derivative structure with interpenetrating
networks. Crystal structure of Bi~3~ Ga Sb~2~ O~11~
;
_journal_coden_ASTM              INOCAJ
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              2314
_journal_page_last               2316
_journal_paper_doi               10.1021/ic50128a019
_journal_volume                  12
_journal_year                    1973
_chemical_formula_structural     'Bi3 Ga Sb2 O11'
_chemical_formula_sum            'Bi3 Ga O11 Sb2'
_chemical_name_systematic        'Tribismuth gallium oxide diantimonate'
_space_group_IT_number           201
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-P 2ab 2bc 3'
_symmetry_space_group_name_H-M   'P n -3 :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.4907(2)
_cell_length_b                   9.4907(2)
_cell_length_c                   9.4907(2)
_cell_volume                     854.9
_refine_ls_R_factor_all          0.051
_cod_original_sg_symbol_H-M      'P n -3 Z'
_cod_database_code               1008051
Crystal and molecular structure of trimercury chloroaluminate, Hg~3~ (Al Cl~4~)~2~
Ellison, R D; Levy, H A; Fung, K W; Inorganic Chemistry 11 (1972) 833–836; doi:10.1021/ic50110a036

data_1008052
_publ_section_title
;
Crystal and molecular structure of trimercury chloroaluminate, Hg~3~
(Al Cl~4~)~2~
;
_journal_coden_ASTM              INOCAJ
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              833
_journal_page_last               836
_journal_paper_doi               10.1021/ic50110a036
_journal_volume                  11
_journal_year                    1972
_chemical_formula_structural     'Hg3 (Al Cl4)2'
_chemical_formula_sum            'Al2 Cl8 Hg3'
_chemical_name_systematic        'Trimercury bis(tetrachloroaluminate)'
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 99.050(3)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.1321(2)
_cell_length_b                   15.0468(3)
_cell_length_c                   14.1771(4)
_cell_volume                     1502.5
_refine_ls_R_factor_all          0.082
_cod_database_code               1008052
La phase Sr La Fe O~4~: Structures cristalline et magnetique
Soubeyroux, J L; Courbin, P; Fournes, L; Fruchart, D; le Flem, G; Journal of Solid State Chemistry 31 (1980) 313–320; doi:10.1016/0022-4596(80)90093-6

data_1008053
_publ_section_title
;
La phase Sr La Fe O~4~: Structures cristalline et magnetique
;
_journal_coden_ASTM              JSSCBI
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              313
_journal_page_last               320
_journal_paper_doi               10.1016/0022-4596(80)90093-6
_journal_volume                  31
_journal_year                    1980
_chemical_formula_structural     'Sr La Fe O4'
_chemical_formula_sum            'Fe La O4 Sr'
_chemical_name_systematic        'Lanthanum strontium iron(III) oxide'
_space_group_IT_number           139
_symmetry_cell_setting           tetragonal
_symmetry_Int_Tables_number      139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.885
_cell_length_b                   3.885
_cell_length_c                   12.784
_cell_volume                     193.0
_exptl_crystal_density_meas      5.94(6)
_refine_ls_R_factor_all          0.018
_cod_database_code               1008053
La phase Sr La Fe O~4~: Structures cristalline et magnetique
Soubeyroux, J L; Courbin, P; Fournes, L; Fruchart, D; le Flem, G; Journal of Solid State Chemistry 31 (1980) 313–320; doi:10.1016/0022-4596(80)90093-6

data_1008054
_publ_section_title
;
La phase Sr La Fe O~4~: Structures cristalline et magnetique
;
_journal_coden_ASTM              JSSCBI
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              313
_journal_page_last               320
_journal_paper_doi               10.1016/0022-4596(80)90093-6
_journal_volume                  31
_journal_year                    1980
_chemical_formula_structural     'Sr La Fe O4'
_chemical_formula_sum            'Fe La O4 Sr'
_chemical_name_systematic        'Lanthanum strontium iron(III) oxide'
_space_group_IT_number           139
_symmetry_cell_setting           tetragonal
_symmetry_Int_Tables_number      139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.878
_cell_length_b                   3.878
_cell_length_c                   12.723
_cell_volume                     191.3
_exptl_crystal_density_meas      5.94(6)
_refine_ls_R_factor_all          0.018
_cod_database_code               1008054
Structure Cristalline du Compose Rb Eu~3~ F~10~
Arbus, A; Fournier, M T; Picaud, B; Boulon, G; Vedrine, A; Journal of Solid State Chemistry 31 (1980) 11–21; doi:10.1016/0022-4596(80)90002-X

data_1008055
_publ_section_title
;
Structure Cristalline du Compose Rb Eu~3~ F~10~
;
_journal_coden_ASTM              JSSCBI
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              11
_journal_page_last               21
_journal_paper_doi               10.1016/0022-4596(80)90002-X
_journal_volume                  31
_journal_year                    1980
_chemical_formula_structural     'Rb Eu3 F10'
_chemical_formula_sum            'Eu3 F10 Rb'
_chemical_name_systematic        'Rubidium trieuropium fluoride'
_space_group_IT_number           225
_symmetry_cell_setting           cubic
_symmetry_Int_Tables_number      225
_symmetry_space_group_name_Hall  '-F 4 2 3'
_symmetry_space_group_name_H-M   'F m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   11.844
_cell_length_b                   11.844
_cell_length_c                   11.844
_cell_volume                     1661.5
_exptl_crystal_density_meas      5.81
_refine_ls_R_factor_all          0.065
_cod_database_code               1008055
La selectivite des substitutions dans les phases MM'P etude de l'ordre par diffraction neutronique dans Ni Co P
Senateur, J P; Rouault, A; L'Heritier, P; Krumbuegel-Nyland, A; Fruchart, R; Fruchart, D; Convert, P; Roudaut, E; Materials Research Bulletin 8 (1973) 229–238; doi:10.1016/0025-5408(73)90176-1

data_1008056
_publ_section_title
;
La selectivite des substitutions dans les phases MM'P etude de l'ordre
par diffraction neutronique dans Ni Co P
;
_journal_coden_ASTM              MRBUAC
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              229
_journal_page_last               238
_journal_paper_doi               10.1016/0025-5408(73)90176-1
_journal_volume                  8
_journal_year                    1973
_chemical_formula_structural     'Ni Co P'
_chemical_formula_sum            'Co Ni P'
_chemical_name_systematic        'Nickel cobalt phosphide (1/1/1)'
_space_group_IT_number           189
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      189
_symmetry_space_group_name_Hall  'P -6 -2'
_symmetry_space_group_name_H-M   'P -6 2 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            3
_cell_length_a                   5.834
_cell_length_b                   5.834
_cell_length_c                   3.351
_cell_volume                     98.8
_refine_ls_R_factor_all          0.015
_cod_database_code               1008056
Structure nucleaire de Ba Ca Fe~4~ O~8~
Herrmann, D; Bacmann, M; Materials Research Bulletin 6 (1971) 725–736; doi:10.1016/0025-5408(71)90106-1

data_1008057
_publ_section_title              'Structure nucleaire de Ba Ca Fe~4~ O~8~'
_journal_coden_ASTM              MRBUAC
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              725
_journal_page_last               736
_journal_paper_doi               10.1016/0025-5408(71)90106-1
_journal_volume                  6
_journal_year                    1971
_chemical_formula_structural     'Ba Ca Fe4 O8'
_chemical_formula_sum            'Ba Ca Fe4 O8'
_chemical_name_systematic        'Barium calcium tetrairon(III) oxide'
_space_group_IT_number           162
_symmetry_cell_setting           trigonal
_symmetry_Int_Tables_number      162
_symmetry_space_group_name_Hall  '-P 3 2'
_symmetry_space_group_name_H-M   'P -3 1 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   5.407(1)
_cell_length_b                   5.407(1)
_cell_length_c                   7.703(3)
_cell_volume                     195.0
_refine_ls_R_factor_all          0.033
_cod_database_code               1008057